Magnetic Nanoparticles - JuSER - Forschungszentrum JÃ¼lich

Magnetic Nanoparticles

A. Feoktystov

This document is a slightly revised version of an article originally published in

Manuel Angst, Thomas Brückel, Dieter Richter, Reiner Zorn (Eds.):

Scattering Methods for Condensed Matter Research: Towards Novel Applications at

Future Sources

Lecture Notes of the 43rd IFF Spring School 2012

Schriften des Forschungszentrums Jülich / Reihe Schlüsseltechnologien / Key **Technologies**,

Vol. 33

JCNS, PGI, ICS, IAS

Forschungszentrum Jülich GmbH, JCNS, PGI, ICS, IAS, 2012

ISBN: 978-3-89336-759-7

All rights reserved.

E 6

Magnetic Nanoparticles

A. Feoktystov

Jülich Centre for Neutron Science

Forschungszentrum Jülich GmbH

Contents

1 Introduction ............................................................................................... 2

2 Magnetic Fluids and their Applications .................................................. 2

2.1 Technical applications ........................................................................................ 3

2.2 Biomedical applications ..................................................................................... 3

3 Magnetic Properties of the Nanoparticles .............................................. 4

3.1 Superparamagnetism .......................................................................................... 5

3.2 Néel relaxation. Blocking temperature ............................................................... 5

4 Small-Angle Neutron Scattering .............................................................. 6

4.1 Contrast variation. Basic functions ..................................................................... 7

4.2 Core-shell structure ............................................................................................. 9

4.3 Polarized neutrons. Magnetic scattering ........................................................... 14

5 Conclusions .............................................................................................. 15

References .......................................................................................................... 16

________________________

Lecture Notes of the 43rd IFF Spring School "Scattering Methods for Condensed Matter Research:

Towards Novel Applications at Future Sources" (Forschungszentrum Jülich, 2012). All rights reserved.

E6.2 A. Feoktystov

1 Introduction

Nowadays materials with nanosized particles are of great interest due to their completely

different properties as compared to the bulk. The knowledge about the behaviour of such

nanomaterials is of great importance. This will give the base for the future development of

substances with the given or controlled properties.

In this lecture we will learn quite new and promising substance – magnetic fluid. As a

research method, the small-angle neutron scattering (SANS) will be presented. A powerful

technique of contrast variation will be discussed in details and applied to small-angle neutron

scattering on magnetic fluids. We will see that small-angle neutron scattering investigations

of magnetic fluids give important information about particle structure and their interaction.

2 Magnetic Fluids and their Applications

Magnetic fluids (or ferrofluids) are colloidal dispersions of magnetic nanoparticles in liquids.

The typical particle size is around 10 nm. The size of the particles is below the critical size, so

that such small particles become single domain in contrast to bulk ferromagnetic material

which has domain structure of magnetization. The single domain nanoparticles have

saturation magnetization. To prevent aggregation of the particles because of the dipole-dipole

interaction (especially under influence of the external magnetic field) particles are usually

coated with a stabilizing surfactant layer [1]. While in the case of non-polar organic carriers

one surfactant layer chemisorbed on the surface of magnetic particles is enough for this

purpose (Fig. 1a), for polar magnetic fluids the double stabilization, conventionally the

formation of the additional second layer, is required [2,3]. In this case, the first layer forms

due to chemisorption of surfactant polar heads on the surface of the magnetic particles. The

second layer is the result of the physical sorption: tails of the second layer’s molecules are

turned to the tails of the first layer’s molecules, thus polar heads of molecules of the second

layer are turned outside, which makes it possible to dissolve the particles in polar carriers.

(a)

(b)

Fig. 1: Schematic representation of nanoparticles in non-polar (a) and polar (b)

magnetic fluid. Note excess of surfactant in solution in case of polar

ferrofluids.

Magnetic Nanoparticles E6.3

Such kind of double-layer stabilization requires some excess of the surfactant molecules in

the solution, so that exchange of molecules of the second stabilization layer with free

molecules in the solvent is in equilibrium (Fig. 1b).

Due to the combination of magnetic properties and liquidity ferrofluids found a large variety

of applications. All the applications are based on the principles that under the influence of

magnetic field the ferrofluid goes to the point where the magnetic field is the strongest,

absorption of electromagnetic energy at convenient frequencies causes the ferrofluid heat up

and the ferrofluid properties can be changed with the application of magnetic field.

2.1 Technical applications

Technical applications consider the ferrofluids’ properties as a whole. In techniques magnetic

fluids are already used in dynamic sealing, damping, bearings, separation, heat dissipation,

measuring devices and so on [4,5]. We will stop here in more details on the applications of

magnetic fluids for heat dissipation and dynamic sealing.

Ferrofluids are used to form liquid seals around the spinning drive shafts in hard disks, which

have to operate in a hermetically closed box because any grain of powder or even smoke may

spoil the reading and writing process. This is achieved by making the hole inside a magnet

and the shaft made of soft magnetic material. A groove in the shaft is filled up with ferrofluid,

which is kept in place by the magnetic field, obstructing the passage of any impurity, but

leaving the axle free to rotate, because the obstructing material is liquid [4,5].

Another good example of ferrofluid application is loudspeaker. Its coil heats up by

functioning and the ferrofluid is kept in place by the magnetic field of the magnet which is

fixed on the loudspeaker’s horn. When the magnetic fluid temperature reaches Curie

temperature, ferrofluid’s particles lose their magnetic properties and a non-magnetic liquid

would flow away and will be substituted by a part of the fluid which has not been overheated.

In this case a passive heat transfer is realized. Nowadays most of the high power loudspeakers

are equipped with ferrofluid. The presence of the fluid around the coil improves also the

quality of the speaker because it damps unwanted resonances, which would produce a very

unpleasant noise [5].

2.2 Biomedical applications

In contrast to technical applications biomedical applications of magnetic fluids focus on the

single colloids’ properties. The main direction of ferrofluids’ application in biomedicine is

cancer treatment. It is magnetic hyperthermia [4,5,6], drug targeting and delivery [5,7],

contrast medium in Magnetic Resonance Imaging (MRI) [5,6,7].

When one applies a drug onto the surface of magnetic particle and focuses the nanoparticles

around cancer tumor with the external magnetic field, the amount of drug necessary is much

less than what would be necessary if it were dispersed in the whole body. When the magnetic

field is turned off the drug will disperse in the body, but, since the total amount is very small,

there will be practically no side effects [5].

The powerful technique of MRI is based on the different relaxation times T 2 of the proton’s

magnetic moments when it is inside different environments. Often the differences are not

strong enough to obtain well resolved images. Dextran coated iron oxides are biocompatible

and are excreted via the liver after the treatment. They are selectively taken up by the

E6.4 A. Feoktystov

reticuloendothelial system. This is important because tumor cells do not have the effective

reticuloendothelial system of healthy cells, so that their relaxation time is not altered by the

contrast agent, which makes them distinguishable from the surrounding healthy cells [5,8].

Hyperthermia is a promising therapy technique which is based on the property of ferrofluids

to absorb electromagnetic energy at a certain frequency. This allows one to heat up a localized

portion of a living body, where ferrofluid has been injected, for example a tumor, without

heating at the same time the surrounding parts of the body. The results of successful

experiments healing cancer tumors in rats and rabbits can be found in [9].

The main problem of Hyperthermia is the high Curie temperature of the used ferromagnetic

materials. The solution is to define substances with low Curie temperature in order to avoid

possible harmful overheating of the human body [10].

3 Magnetic Properties of the Nanoparticles

In bulk ferromagnets the magnetization has a domain structure. These domains form to

minimize the magnetostatic energy of the material. As the size of a magnetic particle is

reduced down to the critical one the magnetic properties of the material are then dictated by

the particle anisotropy and shape rather than by the microstructure of the bulk magnets. There

are two main sources of magnetic anisotropy – magnetocrystalline anisotropy and shape

anisotropy. Magnetocrytalline anisotropy is determined by the atomic structure of a crystal,

which introduces preferential directions for the magnetization (easy axes). The easy and hard

directions arise from the interaction of the spin magnetic moment with the crystal lattice

(spin-orbit coupling). Shape anisotropy appears when a particle is not perfectly spherical. The

demagnetizing field will not be equal for all directions, creating one or more easy axes.

Fig. 2: Coercivity as a function of particle size.

Magnetic Nanoparticles E6.5

Let’s have a look on coercivity as a function of particle size (Fig. 2). For large sizes the

particles are multi-domain becoming more bulk-like with increasing size. Below a critical

particle size domain walls will no longer form due to energy considerations and single domain

particles are stable. This critical size corresponds to the peak in the coercivity in Fig. 2. The

peak position on the particle size axis is dependent on the values of anisotropy and

magnetization. Below the coercivity maximum the particles remain stable until the effects of

temperature destroy the ferromagnetic order. The particles are then superparamagnetic. The

superparamagnetic size strictly depends on the magnetocrystalline anisotropy of the material

[11].

3.1 Superparamagnetism

An assembly of non-interacting single-domain isotropic particles behaves like classical

paramagnetic matter but with very high (~10 3 −10 4 µ B ) effective magnetic moment µ per

particle [12]. If the influence of thermal energy is high enough the magnetic moments of the

nanoparticle are randomized unless a magnetic field is applied. In thermal equilibrium the

average magnetic moment of assemble has the following expression [12]:

(coth( H / kT ) kT / H)

. (1)

Such substances with a huge magnetic susceptibility, whose average magnetic moment is

represented by equation (1), are called then superparamagnetic.

3.2 Néel relaxation. Blocking temperature

Equation (1) is valid only in case of negligible anisotropy energy, but real single-domain

particles are anisotropic. In the normal conditions the magnetization direction inside particle

is along the easy axis. The two states of magnetization of a uniaxial magnetic particle are

separated by an energy barrier (Fig. 3), K u V, where K, is the anisotropy energy density and V

is the particle volume [11]. If the thermal energy, kT, becomes comparable to the barrier

height there is an increased probability of the magnetization reversing.

Fig. 3: Double potential well with two possible orientations of particle magnetic

moment.

E6.6 A. Feoktystov

This thermally activated switching in case of non-interacting single-domain nanoparticles

with the uniaxial magnetic symmetry follow the Née1 relaxation law [12]:

exp( KV

u

)

0

, (2)

kT

where τ is the relaxation time and τ 0 is a constant.

In case of hard disks stability over a time scale of, for example, 10 years gives a stability

criterion of K u V/kT > 40 [13].

The value of τ 0 is typically in the range 10 −13 –10 −9 s [12,14]. The actual magnetic behavior of

nanoparticle assemble depends on the value of the measuring time, τ exp , of the specific

experimental technique with respect to the relaxation time.

If τ exp >> τ, the relaxation is fast and a time average of the magnetization orientation is

observed during the measurement time. In this case the assembly of nanoparticles behaves

like a paramagnetic system. If τ exp

Magnetic Nanoparticles E6.7

received its name. In SANS experiment one registers a dependence of scattering cross-section

(scattering intensity I) on modulus of scattering vector q (i.e. on scattering angle):

4

q sin , (4)

where λ is the neutron wavelength and 2θ is the scattering angle.

The intensity of small-angle neutron scattering is a superposition of particle form- and

structure factors. From the form-factor dependence on the scattering angle one obtains

information about distribution of the scattering density inside scattering particles (size, shape,

etc.). The structure-factor gives information about particle displacement (radial distribution

function).

In 1939 Guinier derived a general expression for the q-dependence of scattering intensity at

small angles, which gives number of scattering parameters directly from scattering curve [15]:

Rq

I( q ~ 0) I(0)exp

3

2 2

g

.

(5)

Here I(0) is called zero scattering intensity and contains information about amount of the

scattering particles and R g is a gyration radius, which as in mechanics is directly connected to

particle dimensions.

4.1 Contrast variation. Basic functions

In contrast to X-ray scattering the amplitude of neutron scattering depends on atomic number

in random way. Thus, for example, it made it possible to detect signal from hydrogen

containing substances of the background of heavy atoms such as iron, copper and so on.

If we consider particles placed in the certain solvent, we have to take into account that the

scattering intensity will not be proportional just to square of the average particle scattering

density but to the square of difference between the average scattering density of the particles

and scattering density of the solvent. This difference is called contrast. If the scattering

densities of the particle and of the solvent are equal the neutrons doesn’t “see” the particles,

since the solution represents a homogeneous continuum, and waves scattered into any

direction will be extinguished. The neutrons give a brilliant possibility to study complex

structures “step-by-step” since one can use hydrogen/deuterium substitution in the solvent or

in some part of the particle. It will significantly change scattering contrast of the system

revealing scattering features that were buried in case of fully protonated system. The idea and

theory of such influence on system contrast was developed by H.B. Stuhrmann and is known

as contrast variation [17].

He showed that scattering intensity can be expanded into series of contrast [17]:

I( q) I ( q) I ( q) ( ) 2 I ( q)

, (6)

s cs c

E6.8 A. Feoktystov

where I s , I cs and I c are called basic functions, Δρ is a contrast. I s gives the residual scattering at

zero contrast – scattering on density fluctuations. I c dominates at high contrasts and represents

thus the scattering intensity of the particle shape. I cs is a cross-term.

The parameters of Guinier approximation (5) have the following dependences (see for

example [18]):

I(0) nV ( )

and

2 2

c

R R ( )

, (7)

2 2

g c

where R c and V c are particle gyration radius and corresponding volume, n particle number

density, α and β are the parameters describing the relative distribution of the “heavy” and

“light” components inside particles [16].

This is only valid for monodisperse non-magnetic particles. In case of polydisperse and

magnetic particles, whose scattering density also depends on size, one has to make averaging

of equation (6) over the particle size distribution function. Nevertheless, as it was shown in

[18] it is still possible to derive the final expression to the same form as (6), but with modified

basic functions and modified contrast:

I q I q I q I q . (8)

2

( )

s( )

cs

( ) ( ) c( )

Here is the modified contrast – the difference between effective average scattering

density of the particles

e

and solvent [18].

Since magnetic scattering doesn’t depend on contrast, its contribution enters into the I

s

modified basic function. Among all of the modified basic functions, which are now the

expressions of classical basic functions, the modified basic function I

c

is just the average of

the classical shape scattering basic function I c over the polydispersity function.

The parameters of Guinier approximation have qualitatively different from (see [18] for more

details):

I(0) n( ) V n ( ) V (2 / 3) n

V

, (9a)

R

2

g

2 2 2 2 2 2

c e c m m

2 2

Vc

Rc

A B D

1

2 2 2

Vc

( )

( )

, (9b)

where ρ m and V m are magnetic scattering density and magnetic volume of the particle, A, B, D

are parameters and denote averaging over polydispersity function. Now it is impossible

to find a scattering density of the solvent which would zero contrast from all of the particles

in solution simultaneously, so there is always residual scattering intensity at the effective

match point (where

0 ): due to polydispersity (the second summand in equation (9a))

and contrast independent magnetic scattering (the third summand in equation (9a)).

Magnetic Nanoparticles E6.9

4.2 Core-shell structure

Magnetic nanoparticles in ferrofluids are of core-shell structure. As an example let’s consider

a simple case of monodisperse non-magnetic nanoparticles (Fig. 4).

Fig. 4: Schematic representation of the particle core-shell structure.

0

and

1

are

scattering densities of the particle core and shell ( ( V0 V1 ) 0 (1 V0 V1 ) 1

is the average particle scattering density),

s

is solvent scattering density. R 0

and R 1 are the radii of particle core and shell.

The expression for scattering intensity in this case consists of the core and shell contributions:

I( q) n[( ) V ( qR ) ( ) V ( qR )]

2

1 s

1 1

1 0 0 0

, (10)

where V 0 and V 1 are the particle and “particle+shell” volumes and Φ(x) is the spherical

3

scattering amplitude: ( x) 3(sin x xcos x) / x [16].

Combining the members at contrast s

, the three basic functions in equation (6) can

be derived analytically:

I ( q)

nV ( ) [ ( qR ) ( qR )] , (11a)

s

2 2 2

0 1 0 1 0

I ( q) 2 nVV ( ) ( qR )[ ( qR ) ( qR )]( )

, (11b)

cs

1 0 1 0 1 1 0

2 2 2

I ( c

q ) nV ( )( )

1

qR1

. (11c)

To obtain the three basic functions one has to measure scattering curves for at least three

contrasts, then the system of equations of type (6) can be easily solved and compared to the

analytical result.

In case of magnetic nanoparticles one has to add a magnetic contribution in equation (10), the

square of magnetic form-factor F M :

F ( q) [ V ( qR )] . (12)

2 2

M m m m

E6.10 A. Feoktystov

In case of SANS with non-polarized neutrons on diluted unmagnetized samples of ferrofluids,

the total scattering intensity contains contributions of nuclear form-factor and 2/3 of magnetic

form-factor (for more details refer to [19]):

2 2 2

I( q) FN( q) FM( q)

. (13)

3

As a first example we consider organic magnetic fluids which are polydisperse magnetite

(Fe 2 O 3 ) nanoparticles coated with a single layer of oleic (OA) or myristic acid (MA) in

benzene [20].

Intensity, cm -1

10

1

0.1

0.01

0.1 1

100% C 6

D 6

10% C 6

D 6

90% C 6

D 6

20% C 6

D 6

75% C 6

D 30% C

6

10

6

D 6

60% C 6

D 50% C

6

6

D 6

50% C 6

D 6

55% C 6

D 6

40% C 6

D 60% C

6

6

D 6

1

38% C 6

D 70% C

6

6

D 6

35% C 6

D 6

32% C 6

D 6

75% C 6

D 6

90% C 6

D 6

30% C 6

D 6

0.1

20% C 6

D 6

10% C 6

D 6

0.01

-1 0.1 1

Intensity, cm -1

(a)

(b)

Fig. 5: Contrast variation curves of SANS on diluted ferrofluids: (a) – MA

stabilization, (b) – OA stabilization. The amount of D-benzene in the solvent

(i.e. contrast) is indicated in the legend.

For changing system contrast initial concentrated magnetic fluids (based on C 6 D 6 ) were

diluted with different mixtures of D- and H-benzene, so that the D-benzene content in the

final solution was varied within interval 10-100 % (10–12 points). The final magnetic particle

concentrations in ferrofluids were 0.8 % and 0.7 % in case of MA and OA stabilization

respectively. The whole set of obtained scattering curves at different contrast are presented in

Fig. 5.

To each of the scattering curves in Fig. 5 the Guinier approximation (5) was applied and the

dependences (9) were obtained (Fig. 6):

100% C 6

D 6

Magnetic Nanoparticles E6.11

I(0) for OA, cm -1

35

30

25

20

15

10

5

0

34.2 %

OA

MA

63 %

0

0.0 0.2 0.4 0.6 0.8 1.0 1.2

[C 6

D 6

]/[C 6

D 6

+C 6

H 6

]

10

8

6

4

2

I(0) for MA, cm -1

R 2 g , nm2

80

70

60

50

40

30

20

10

0

-10

OA

MA

-18-16-14-12-10 -8 -6 -4 -2 0 2 4 6 8 10

() 10 -10 , cm 2

/

(a)

(b)

Fig. 6: The parameters of the Guinier approximation (5) fitted according to equations

(9). (a) – zero scattering intensity dependence on deuteration of the solvent and

(b) – dependence of gyration radius on inversed contrast.

The effective match points were determined from parabolic fitting of curves in Fig. 6a as

34.2 ± 0.4 % and 63 ± 3 % of the D-benzene content for MA and OA fluids, respectively. The

corresponding scattering density’s values are (2.64 ± 0.03) × 10 10 cm -2 and (3.86 ± 0.15) ×

10 10 cm -2 . Taking into account the quasi-spherical shape of particles in magnetic fluids the

characteristic radius of the whole particle was calculated from the fit results were calculated

to be 5.0 ± 0.1 nm (MA) and 10.3 ± 0.1 nm (OA) [20]. Thus, combining the results of the

calculated effective match point, which shows that OA sample contains more of heavier

component (magnetite) in the particles, and radius of the particles one can speak about size

regulation effect when using such two surfactants to synthesize the ferrofluids. The particle

size, which comprises both the mean size and polydispersity, in OA fluid is twice larger as

compared to MA fluid.

From the whole set of scattering curves the three basic functions from equation (8) were

calculated. The best way to check the reliability of the calculated basic functions is to

compare I s basic function, which is a residual scattering intensity at zero contrast, with the

scattering curve close to math point (Fig. 7). As one can see, the I s basic functions coincide

well with measured SANS curves which confirms correctness if the basic function separation.

Comparison of the shape scattering basic functions I c for two magnetic fluids directly

confirms the results of fit of gyration radius dependence on inversed contrast in Fig. 6b with

the expression (9b). The I c basic function in case of OA stabilization is more steep than MA

sample, which is the results of larger particles in the ferrofluid.

E6.12 A. Feoktystov

1

MA

MA 35% C 6

D 6

OA

OA 60% C 6

D 6

10 MA

OA

1

0.1

I s

, cm -1

I c

, x10 -20 cm 3

0.1

0.01

1E-3

0.1 1

1E-4

0.1 1

q, nm -1 q, nm -1

(a)

(b)

Fig. 7: Calculated basic functions of expression (8). (a) represents I s basic function of

the residual scattering and (b) – I c shape scattering basic functions. I cs is not

shown due to the lack of its transparent interpretation.

For the next example we consider water-based magnetic fluids. Performing the same steps for

sample dilution with different ratios of H 2 O and D 2 O as for previous ferrofluids the SANS

contrast variation curves were measured in 10 contrast points for each sample (Fig. 8) [21,22].

Intensity, cm -1

100

10

1

0.1

0% D 2

O

10% D 2

O

20% D 2

O

30% D 2

O

40% D 2

O

50% D 2

O

60% D 2

O

70% D 2

O

80% D 2

O

90% D 2

O

Intensity, cm -1

10

1

0.1

0% D 2

O

10% D 2

O

20% D 2

O

30% D 2

O

40% D 2

O

50% D 2

O

60% D 2

O

70% D 2

O

80% D 2

O

90% D 2

O

0.01

0.1 1

0.1 1

q, nm -1 q, nm -1

(a)

(b)

Fig. 8: SANS contrast variation curves for water-based magnetic fluids with double

layers of lauric (LA) (a) and myristic acid (MA) stabilization (b). The ration of

D 2 O in the solvent is indicated in the legend.

As one can see, Guinier region, which is represented by a plateau at small q-values, is

inaccessible here due to an aggregation in ferrofluids. The water-based magnetic fluids

require double stabilizing shell around magnetic nanoparticles. The second layer is quite weak

and its molecules are in equilibrium with the free surfactant in the solvent. The equilibrium is

very sensitive to external actions and such ferrofluids are usually characterized by the

existence of aggregates (see for example [23]).

Magnetic Nanoparticles E6.13

Nevertheless, the three basic functions (8) were calculated, among them the most informative

shape scattering basic function I c (Fig. 9a). From the more steep I c curve of LA magnetic fluid

one can easily say that particles (aggregates) in the sample are large than in MA sample.

10

1

0.1

LA

MA

0.25 TEM of separate particles

0.20

Indirect Fourier Transform of I c

(q)

MA

Indirect Fourier Transform of scattering

curve of the sample on H 2

O

0.15

LA

I c

, x10 -20 cm 3

p(r)

0.01

1E-3

0.1 1

0.10

0.05

0.00

0 10 20 30 40 50

q, nm -1 r, nm

(a)

(b)

Fig. 9: Shape scattering basic functions for both ferrofluids. Line shows fit according

to Indirect Fourier Transformation [24] (a). The pair distance distribution

functions calculated from the shape scattering basic functions, scattering

curves of the samples in pure H 2 O and compared to the results of Transmission

Electron Microscopy measurements [22] (b).

The comparison of pair distribution functions calculated from I c basic function and scattering

curves of ferrofluids on H 2 O, where due to a weak contrast between shell and water the

scattering originates mainly from magnetite core, are compared to the results of Transmission

Electron Microscopy, when only single particles were taken into account (Fig. 9b). In both

cases experimental curves give broader p(r) function pointing to the existence of large

aggregates in the samples. In case of LA sample the maximum r-value of p(r) functions are

different on 7 nm. This can be associated with shell (~3.5 nm) around the particles which is

apparent in I c function, but not in scattering on H 2 O-based sample. In MA sample the p(r)

functions coincide, so in this sample the aggregates consist of nanomagnetite with one

incomplete layer of the surfactant [21,22].

In case of maghemite water-based ferrofluid stabilized by short citric ions (charge

stabilization [25]) the particles can be considered as homogeneous [26]. The Coulomb

interaction is compensated with the addition of NaCl to the solvent. In that case, the result of

SANS contrast variation experiment gives directly two characteristic sizes of the particles –

nuclear and magnetic [18]. The dependence of the gyration radius on contrast together with its

fit is presented in Fig. 10.

The difference in magnetic and nuclear radii of around 3 nm could hardly be explained as the

existence of magnetically dead layer on the edge of maghemite nanoparticles in the ferrofluid.

As it was shown such a difference can be explained as a result of non-uniform charge

distribution on the surface of the particles and as a result the existence of residual Van der

Waals interaction (for more details refer to [26]).

MA

LA

E6.14 A. Feoktystov

Fig. 10: The dependence of the gyration radius on contrast and its fit according to [18].

4.3 Polarized neutrons. Magnetic scattering

When polarised neutrons are used with the neutron spins aligned antiparallel (+) or parallel

(−) to the direction of an applied magnetic field H scattering intensity depends on the neutron

spin state [27,28,19]:

I ( q) F ( q) [ F ( q) 2 F ( q) F ( q)]sin

, (14a)

2 2 2

N M N M

I ( q) F ( q) [ F ( q) 2 F ( q) F ( q)]sin

, (14b)

2 2 2

N M N M

where φ is azimuthal angle in detector plane.

(a)

(b)

Fig. 11: Separation of nuclear and magnetic scattering contributions for magnetite

ferrofluids based of deuterated cyclohexane and stabilized with oleic (a) and

myristic acid (b).

Magnetic Nanoparticles E6.15

Thus, character of the scattering is anisotropic now. By making cuts of scattering pattern for

both intensities in sectors 0° with 180° and 90° with 270° and solving the system of equations

(14) one can separate nuclear F N and magnetic F M contributions [29,30]. Separation of nuclear

and magnetic scattering on the example of organic ferrofluid is represented in Fig. 11.

Different magnetic and nuclear radii calculated from Guinier approximation point to a

complex correlation between the magnetic moments of the particles. These correlations differ

qualitatively for the two samples [30].

When a polarization analysis of the scattered beam is applied four types of scattering

processes are distinguished, two for conserving the neutron spin (F ++ ) 2 and (F −− ) 2 (non spin

flip scattering, NSF) and two with reversal of the spin with the scattering (F +− ) 2 and (F −+ ) 2

(spin-flip scattering, SF) [27,28,19]. In a particle of radius 4 nm, about 50 % of atoms lie on

the surface. The concept of a well-defined super-moment breaks down. Single domain

nanoparticles still have uniform magnetization direction, but their spin configuration is not so

transparent [31]. In real particles, the surface region thickness is very sensitive to particle

shape distortion, surface roughness, surface impurities, defects (like vacancies),

compositional inhomogeneity, surface chemical bonds with environment, etc [12]. In

literature one can find several possible descriptions of particle spin configuration (see for

example [32]).

For the first time the magnetically distinctive core-shell morphology was “seen” in the work

[33], where the polarization analysis was successfully applied to directly extract the average

spatial distributions of magnetic moments and their correlations. From the obtained scattering

in perpendicular direction to the applied magnetic field the authors conclude that magnetic

shells of nearly uniform magnitude and direction around the magnetic core exist.

5 Conclusions

Magnetic nanoparticles in general and magnetic fluids particularly nowadays are widely used

in technics and are very promising for biomedical applications. For the latter case structure

and properties of the substances have to be known beforehand in order to control the synthesis

process. The small-angle neutron scattering together with contrast variation technique plays a

crucial role in particle structure definition. The newly developed approach of basic functions

in contrast variation experiments for the case of polydisperse magnetic nanoparticles opens

new possibilities for structural determination. Compared to the monodisperse case, the

contrast dependence of scattering integral parameters for the polydisperse system contains a

number of additional parameters comprising information about polydispersity function of the

system; their analysis increases the reliability of experimental results. As to the SANS data

fitting according to supposed particle models the contrast variation technique results in

additional parameters, which can be included in the fit function as constants, thus reducing the

number of free parameters and increasing the reliability of the fit.

Acknowledgements: the author would like to thank colleagues without whom this work

would have not been possible: M.V. Avdeev, V.L. Aksenov (FLNP JINR, Russia),

L.A. Bulavin, V.I. Petrenko (Physics Department KNU, Ukraine), L. Vekas, D. Bica [1952-

2008], O. Marinica (Laboratory of Magnetic Fluids CFATR, Romania), V.M. Garamus,

R. Willumeit (HZG, Germany), E. Dubois, R. Perzynski (UPMC, France).

E6.16 A. Feoktystov

References

[1] R.E. Rosensweig, Ferrohydrodynamics, Cambridge University Press 1985.

[2] D. Bica, L. Vekas, M.V. Avdeev, et al.: J Mag Mag Mater 311 (2007) 17-21.

[3] M.V. Avdeev, V.L. Aksenov, M. Balasoiu, et al., J Coll Interface Sci 295 (2006) 100-107.

[4] S. Odenbach (Ed.), Colloidal Magnetic Fluids: Basics, Development and Application of

Ferrofluids, Lect. Notes Phys. 763, Springer, Berlin Heidelberg 2009.

[5] C. Scherer, A.M. Figueiredo Neto, Braz J Phys, 35(3A) (2005) 718-727.

[6] N.A. Brusnetsov, T.N. Brusnetsova, E.Yu.Filinova, et al., J Mag Mag Mater 311 (2007)

176-180.

[7] C. Sun, J.S.H. Lee, M. Zhang, Advanced Drug Delivery Reviews 60(11) (2008) 1252-

1265.

[8] Q.A. Pankhurst, J. Connolly, S.K. Jones and J. Dobson, J Phys D Appl Phys 36 (2003)

R167-181.

[9] N.A. Brusentsov, L.V. Nikitin, T.N. Brusentsova, et al., J Mag Mag Mater 252 (2002)

378-380.

[10] T.N. Brusentsova, V.D. Kuznetsov, J Mag Mag Mater 311 (2007) 22-25.

[11] D. Sellmyer, R. Skomski (Eds.), Advanced Magnetic Nanostructures, Springer 2006.

[12] S.P. Gubin (Ed.), Magnetic Nanoparticle, WILEY-VCH Verlag GmbH & Co. KGaA,

Weinheim 2009.

[13] C.A. Ross, Annu Rev Mater Res 31 (2001) 203-235.

[14] J.L. Dormann, D. Fiorani, E. Tronc, Magnetic Relaxation in Fine-Particle Systems, in

I. Prigogine, S.A. Rice (Eds.), Adv Chem Phys 98, John Wiley & Sons, Inc., Hoboken, NJ,

USA 2007.

[15] G. Porod, General Theory, in O. Glatter, O. Kratky (Eds.), Small Angle X-ray Scattering,

Academic Press Inc. (London) Ltd., 1982.

[16] L.A. Feiging, D.I. Svergun, Structure Analysis by Small-Angle X-Ray and Neutron

Scattering, Plenum Press, New York 1987.

[17] H.B. Stuhrmann, Contrast Variation, in O. Glatter, O. Kratky (Eds.), Small Angle X-ray

Scattering, Academic Press Inc. (London) Ltd., 1982.

[18] M.V. Avdeev, J Appl Cryst 40 (2007) 56-70.

[19] A. Wiedenmann, Physica B 356 (2005) 246-253.

[20] A.V. Feoktystov, M.V. Avdeev, V.L. Aksenov, et al., Solid State Phenom 152-153 (2009)

186-189.

[21] A.V. Feoktystov, L.A. Bulavin, M.V. Avdeev, et al., Ukr J Phys 54 (2009) 266-273.

[22] M.V. Avdeev, B. Mucha, K. Lamszus, et al., Langmuir 26(11) (2010) 8503-8509.

[23] M.V. Avdeev, V.L. Aksenov, M. Balasoiu, et al., J Coll Interface Sci 295 (2006) 100-107.

[24] J. Skov Pedersen, Adv Coll Interface Sci 70 (1997) 171-210.

[25] R. Massart, E. Dubois, V. Cabuil and E. Hasmonay, J Magn Magn Mater 149 (1995) 1-5.

[26] M.V. Avdeev, E. Dubois, G. Mériguet, et al., J Appl Cryst 42 (2009) 1009-1019.

[27] R.M. Moon, T. Riste, W.C. Koehler, Phys Rev 181(2) (1969) 920-931.

[28] R. Pynn, J.B. Hayter, S.W. Charles, Phys Rev Lett 51 (1983) 710-713.

Magnetic Nanoparticles E6.17

[29] M.V. Avdeev, M. Balasoiu, V.L. Aksenov, et al., J Magn Magn Mater 270 (2004) 371-

379.

[30] M. Balasoiu, M.V. Avdeev, A.I. Kuklin, et al., Rom Rep Phys 58(3) (2006) 305-311.

[31] R.A. Kodama, A.E. Berkowitz, Phys Rev B 59 (1999) 6321-6336.

[32] Y. Labaye, O. Crisan, L. Berger, et al., J Appl Phys 91 (2002) 8715-8717.

[33] K.L. Krycka, R.A. Booth, C.R. Hogg, et al., Phys Rev Lett 104 (2010) 207203.